## Calculations of electronic band structure and optical properties of HgTe

## under pressure

P K Sainia, b_{*, D Singh}c_{ & D S Ahlawat}a

a_{Department of Physics, Chaudhary Devilal University, Sirsa 125 055, India }
b_{Department of Physics, Government P G College, Hansi 125 033, India }

c_{Department of Physics, M M University, Ambala 133 203, India }

*Received 17 March 2017; accepted 21 May 2017 *

The electronic band structure and optical properties of HgTe have been reported using the full potential linearized augmented plane wave (FP-LAPW) method based on density functional theory. In this approach, generalized gradient approximation (GGA) and Engel-Vosko generalized gradient approximation (EV-GGA) have been used for the exchange correlation potential in the calculations. The electronic band structures have been calculated to discuss the electronic properties and optical properties of the compound. Moreover, optical properties including dielectric functions, absorption, optical conductivity, refractive index, reflectivity and energy loss spectrum have been obtained and analyzed in details within the energy range up to 14 eV. The obtained results have been compared with the previous calculations and available experimental data. Overall good agreement is found.

**Keywords: Electronic band structure, Elastic constants, Optical properties, WIEN2k **

**1 Introduction **

Recently, there has been much interest in various properties of II-VI binary semiconductor compounds and alloys1-4. Among these materials, HgX (where X= S, Se and Te) compounds are found to be very important materials due to their technological applications particularly in optoelectronics devices. There have been several experimental and theoretical studies on this materials5-9. Although density-functional theory DFT methods have proved important for studying high-pressure phases10, only a few such studies of mercury chalcogenides have been reported up to now11-13. In this paper we have presented the results of a first-principles DFT study of electronic band structure and optical properties of the zinc blende and rocksalt structure of HgTe, to the best of our knowledge, have not been considered theoretically before, particularly at high pressure. In addition to this work, we also have discussed the common trends and the differences in band structures and optical properties of HgTe at ambient and high pressure.

**2 Method of Calculation **

The calculations are performed using the scalar relativistic FP-LAPW approach within DFT, as

implemented in the WIEN2K code14. The
exchange-correlation energy of electrons is described in the
generalized gradient approximation (GGA) within the
parameterization of Perdew-Burke-Ernzerhof15,16 (PBE)
to calculate the total energy. Moreover, the
Engel-Vosko generalized gradient approximation (EV-GGA)
formalism is also applied so as to optimize the
corresponding potential for electronic band structure
calculations in order to improve the band gap17.
In these calculations, the unit cell was divided
into two regions. The spherical harmonic expansion
was used inside the non overlapping spheres of
*muffin-tin radius (R*MT) and the plane wave basis set

was chosen in the remaining space of the unit cell
*(interstitial region). The R*MT for Hg and Te were

chosen for the expansion of the wave functions in the
interstitial region in such a way that the spheres
did not overlap. The basis functions in the
*interstitial region were expanded up to R*MT**K*MAX = 7.0

inside the atomic spheres for the wave function
to get the total energy convergence. The maximum
*value of l was taken as l*max = 10 in the muffin-tin

spheres, while the charge density is Fourier expanded
*up to G*max = 14 a.u-1. The atoms are taken at the

positions of Hg(0,0,0) and Te(1/4,1/4,1/4) for ZB
phase and Hg(0,0,0) and Te(1/2,1/2,1/2) for RS
phase of HgTe, respectively. Accurate convergence
**——————— **

criteria have been considered for all the above mentioned parameters.

**3 Results and Discussion **

**3.1 Band structure **

The calculated total energies are fitted according to
Murnaghan equation of state18 (EOS) to obtain the
equilibrium lattice constant. The optimized lattice
constant of HgTe is obtained as 6.67 Å in zinc blend
phase whereas it is found 5.78 Å for RS phase under
the application of high pressure at about 17.09 GPa.
Using these equilibrium lattice parameters, we have
calculated and plotted the band structure at ambient
pressure ZB phase as well as high pressure RS phase
of HgTe by use of FP-LAPW method with in EV-GGA
scheme. The derived electronic band structures were
further used to study other properties like band gap and
optical properties etc. The electron dispersion curves
along the high symmetry directions in the brillouin
zone for zinc blende and rocksalt phase of HgTe are
plotted in Fig. 1(a) and 1(b) within the EV-GGA
*schemes, respectively. The Fermi level (E*F) was

selected to position at 0 eV and coincides with the top
of the valence band. The calculated band structure
profiles for both the phases have been found similar.
However, a little difference in the band location on
energy scale may be seen as in the case of ambient
phase. It can be seen that the lowest lying band in the
valence band region are positioned at –11.0 eV for both
the phases. It mainly arises from the s states of Te
*while the bands in valence region just below E*F

*are predominantly due to s and p orbital of Hg. *
*The conduction band above E*F is mainly due to d states

*of Hg which hybridize with p and d states of Te. *
Similarly, the electron dispersion curves along the
high symmetry directions for high pressure rock salt
(B1) phase of HgTe is plotted and analyzed in
Fig. 1(b). The band structure of B1 phase of HgTe by
FP-LAPW method has also not been reported to the
best of our knowledge. It can be seen that the
lowest-lying band in the valence band region mainly arises
*from the s states of Te while the bands in valence *
*region just below E*F* are predominantly due to s and *

*p orbital of Hg. The conduction band above E*F is

*mainly due to d states of Hg which hybridize with *
*p and d states of Te. Furthermore, as we can see *
from the figure, in high pressure rock salt (B1)
phase of HgTe, this hybridization interaction of the
*d electrons with anion p electrons leads to a repulsion *
of the involved states. An increased width of the upper
valence bands and a decrease in the band gap has been
*observed. The later may occur because of Te- p states *
*are pushed up in energy towards the Hg -s derived *
*conduction bands by p-d interaction. Therefore the *
*d bands show remarkable dispersion and separate *
against in two groups of bands. When there is stronger
*p-d interaction in HgTe then there is increase in the *
*d band width. The metallic character increases under *
high pressure RS phase due to crossing of conduction
band at Fermi level in different high symmetric
directions in band structures. Thus, comparing
LAPW-EV-GGA calculations in the zincblende and rock salt

Fig. 1 – (a) Band structure of HgTe in zinc-blende phase using EV-GGA and (b) band structure of HgTe in rocksalt phase using EV-GGA

phases, one see that the band structures are very
**similar, except the bandgap at Г point. The calculated **
value of band gap for ZB phase using EV- GGA
schemes are shown in the Table 1 along with the
previous theoretical reported work19_{ and experimental }

values20,21_{. Our calculated band structure of HgTe }

indicate a negative direct band gap equal to –0.543 eV and has been found in good agreement with the available experimental results.

**3.2 Optical properties**

The optical properties are obtained from the
complex dielectric function αβ *(ω) = Re *αβ **(ω) + i Im **

αβ (ω) = 1*(ω) + i*2(ω), which is related mainly to the

electronic structure of solid. The imaginary part 2(ω)

of the dielectric function is calculated from the total density of states and the momentum matrix elements between the occupied and unoccupied Eigen states of the material. The real part 1(ω) of the frequency

dielectric function can be computed from 2(ω)

using the Kramer-Kronig relationship22,23_{. Using the }

dispersion of real and imaginary parts of dielectric functions one can calculate dispersion of other optical parameters such as, optical conductivities, absorption

coefficient, reflectivity, dielectric constant, refractive index, extinction coefficient and eloss function. Figure 2(a) displays the dispersion of the real and imaginary parts of dielectric function, 1(ω) and 2(ω),

for ZB HgTe. The observed spectra 2(ω) show the

threshold energy occurring at 0.12 eV. It may be seen that the three major energy spectral peaks situated at 2.01, 3.9 (principal peak), and 6.21 eV. The maximum peak height in ε2(ω) at about 2.01 eV is lying at 13.3,

which corresponds to the transition from occupied
*Hg-s to unoccupied Te-Hg-s band Hg-stateHg-s. The calculated Hg-static *
dielectric constant ε1(0) without any contribution from

lattice vibration is equal to about 18.4 as shown in Fig. 2(a) The wide band energy gap yields a smaller value of ε1(0). Our calculated value of static dielectric

constant is presented in Table 2. It may be observed that a smaller energy gap yields a larger 1(0) value.

Figure 2(b) displays the calculated real 1(ω) and

imaginary dielectric function 2(ω) for the RS HgTe

compound. It may be seen that the 2(ω) shows a large

peak (positioned at 2.3 eV) for HgTe for the RS phase. Figure 3(a) displays the calculated absorption spectrum α(ω), for the HgTe compound in ZB phase and RS phase. The absorption edge starts at about 0.19 eV in the spectrum. The absorption spectrum α(ω), shows a very intense absorption at about 6.49 eV, which may be due to excitations of photons. In case Table 1 – Calculated direct-band gap for zinc blende phase of

HgTe along with the other theoretical and experimental work

Material Calculations Direct band gap(eV)
at Г point
HgTe
Present work
(using EV-GGA) -0.543
Theorya _{-0.84 }
Experimentalb _{-0.30 }
Experimentalc _{-0.3 }
a_{Ref}19_{, }b_{Ref}20_{, }c_{Ref}21

Fig. 2 – (a) Real 1(ω) and imaginary 2(ω) dielectric function of ZB HgTe and (b) real and imaginary 2(ω) dielectric function of RS HgTe

Table 2 – Calculated values of static dielectric constant for zincblende and rocksalt phases of HgTe

Compound Phase Calculation Static dielectric constant, ε1(0)

HgTe ZB Present work 18.4

Others -

RS Present work 30.2

of RS phase, the absorption edge starts at about 0.67 eV in the spectrum. The highest peaks located in the spectrum are due to the transition of electrons along high symmetry directions. It was observed that the occupied electron states are excited to unoccupied electron states in upper Fermi level by absorbing photons or by application of high pressure. This inter-band transition is called optical conduction also known as Drude transition. The spectrum in Fig. 3(b) shows that the optical conduction starts with energy of about 0.22 eV and 0.98 eV for ZB and RS phases of HgTe, respectively. The optical conductivity is found to be increased with the increase of photon energy. After attaining the maximum value of optical conductivity at 6.5 eV for ZB and 2.3 eV for RS phase, it starts to decrease with increase of photon energy. The excited electrons have no enough energy to pass the energy gap, and transfer to the conduction band. Thus, the band gap energy is the main reason of starting optical conduction σ(ω).

Further, Fig. 4(a) shows the calculated frequency
*dependent reflectivity R(ω) for the HgTe compound in *

ZB and RS phase. A strong reflectivity maximum has been observed between the energy range 6.2 eV– 10.3 eV and 2.1 eV–3.3 eV for ZB and RS phase, respectively, which may be arises due to the inter-band transitions. Further, A strong reflectivity minimum is seen at energies ranging from about 8.1–10 eV and 5.2–10.6 for ZB and RS phase, respectively, which representing a collective plasma resonance. The depth of the plasma minimum can be calculated by the imaginary part of the dielectric function at the plasma resonance and gives the degree of overlap between the inter-band absorption regions. The calculated refractive index for the ZB and RS HgTe compound are shown in Fig. 4(b). It can be noticed that the refractive index is significant only up to 1.7 eV for ZB and 1.62 eV for RS phase, beyond these energy range it drops sharply. The theoretically calculated static refractive index 4.3 for ZB and 5.5 for RS HgTe are displayed in Table 3. There are no experimental and theoretical results available on refractive index in the literature for comparison of our calculated values of refractive index of ZB and RS HgTe. The electron

Fig. 3 – (a) Absorption α(ω) of HgTe in ZB and RS phase and (b) optical conductivity of HgTe in ZB and RS phase

energy loss spectroscopy (EELS) is very useful technique for investigating various aspects of study for the materials including non-scattered and elastically scattered electrons (zero Loss). The energy losses are mainly due to a complicated mixture of single electron excitations and collective excitations (plasmons) at some intermediate energy range (typically 1 to 50 eV). The single electron excitation peaks positions are related to the joint density of states between the conduction and valence bands, whereas the energy required for the excitation of bulk plasmons depends on the electron density. The electrons, which are responsible to excite the atomic electrons of the outer shell is called valence loss or valence intera-band transitions. Inter-band transitions consist mostly of plasmon excitations and the scattering probability for volume losses is directly associated to the energy loss function. Figure 5(a) shows that the most prominent peak in the energy loss spectrum is associated with the Plasmon peak and located at 11 eV for ZB phase and 12.1 eV for RS phase of HgTe. The corresponding frequency associated to Plasmon peak is called plasma frequency24,ωp.

*The extinction coefficient k(ω) is calculated and *
plotted in Fig. 5(b) of HgTe for both ZB and RS phase,
respectively. The local maxima of the extinction
*coefficient k(ω) corresponds to the zero of * 1(ω)

(6.1 eV) for HgTe in ZB phase and 2.2 eV for HgTe in

RS phase, respectively. The difference in the spectra of the extinction coefficient for ZB and RS indicates that there is a shifting of the maxima peak towards lower energy side for RS and increase in peak height. To the best of our knowledge, we have not found any experimental and theoretical data available in the literature especially at high pressure RS phase to compare our results of HgTe for optical dispersions. However, the calculated results of optical dispersion may be helpful for future predictions about HgTe compound at ambient as well as high pressure RS phase and perform more suitable experiments in this direction for further research work on this material.

**4 Conclusions **

In this work we have studied the band structure and optical properties of HgTe compound using the first principles calculations. The calculated results for electronic band structures show that these compounds have inverted band structures. It is also observed that HgTe compound having semi-metallic nature in ZB phase. The metallic character is found to be increased under high pressure RS phase due to crossing of conduction band at Fermi level in different high symmetric directions in band structures. The theoretically obtained values of static dielectric constants 1(0) and static refractive index are found to

be increased with the increasing metallic behavior of the compound. Furthermore, we have also calculated the other optical properties like dielectric function, absorption, optical conductivity, reflectivity, refractive index, eloss function and extinction coefficient for ZB and RS HgTe in details. The calculated results could be useful for further experimental investigations about this compound.

Fig. 5 – (a) Eloss function of HgTe in ZB and RS phase and (b) extinction coefficient of HgTe in ZB and RS phase

Table 3 – Calculated static refractive index for zincblende and rocksalt phases of HgTe

HgTe Calculations Static refractive index

ZB phase Present work 4.3 Others - RS phase Present work 5.5 Others -

**References **

1 *Corso A D L, Baroni S, Resta R & Girononcoli S de, Phys *

*Rev B, 47 (1993) 3588. *

2 *Jain M, II-VI Semiconductor compounds, (World Scientific, *
Singapur) 1993.

3 *Chen A B & Sher A, J Vac Sci Technol, 21 (1982) 138. *
4 *Cervantes P, Williams Q, Oleg C M & Cohen M L, Phys Rev *

*B, 54 (1996) 17585. *

5 *Sun S R & Dong Y H, Phys Rev B, 72 (2005) 174101. *
6 *Boutaiba F, Zaoui A & Ferhat M, Superlattice Microstruct, 46 *

(2009) 823.

7 *Verma A S, Singh R K & Rathi S K, Physica B, 404 (2009) *
4051.

8 Cardona M, Kremer R K, Lauck R, Siegle G, Muñoz A &
*Romero A H, Phys Rev B, 80 (2009) 195204. *

9 *Kumar V, Shrivastava A K & Jha V, J Phys Chem Solids, 71 *
(2010) 1513.

*10 Mujica A, Rubio A, Muñoz A & Needs R J, Rev Mod Phys, *
75 (2003) 863.

*11 Lu Z W, Singh D & Krakauer H, Phys Rev B, 39 (1989) 10154. *
*12 Sun S R & Dong Y H, Phys Rev B, 72 (2005) 174101. *

*13 Fleszar A & Hanke W, Phys Rev B, 71 (2005) 045207. *
14 Blaha P, Schwarz K, Madsen G K H, Kvasnicka D & Luitz J,

*An augmented plane wave plus local orbitals program for *
*calculating crystal properties, Vienna University of *

Technology, Vienna, Austria, 2001.

15 Perdew J P, Chevary J A, Vosko S H, Jackson K A, Pederson
*M R, Singh D J & Fiolhais C, Phys Rev B, 46 (1992) 6671. *
16 Peterson M, Wanger F, Hufnagel L, Scheffler M, Blaha P &

*Schwarz K, Comput Phys Commun, 126 (2000) 294. *
*17 Engel E & Vosko S H, Phys Rev B, 47 (1993) 13164. *
*18 Murnaghan F D, Proc Natl Acad Sci USA, 30 (1944) 244. *
*19 Chen X, A Mintz, Hu J, Hua X & Zinck J, J Vac Sci *

*Technol B, 13 (1995) 4. *

*20 O Madelung & Landolt B, Numerical data and functional *

*relationships in science and technology, (Springer: Berlin), *

1982.

*21 Strehlow W H & Cook E L, J Phys Chem, 2 (1973) 163. *
*22 Kiang L L, Chinese J Phys, 14 (1976) 93. *

*23 Wooten F, Optical properties of solids, (Academic Press: *
New York), 1972.